Study on Macro-Meso Deformation Law and Acoustic Emission Characteristics of Granular Gangue under Different Loading Rates
2. Experimental Design and the Establishment of Particle Flow Numerical Model
2.1. Material Preparation
2.2. Experiment Design
2.3. Construction of Particle Flow Numerical Model
3. Result and Analysis
3.1. Confined Compression Deformation of Gangue at Different Loading Rates
- Stress-strain relationship
- The overall trend of stress–strain curves of gangue specimens under six different loading rates is consistent. With the increase of stress, the strain presents three stages of fast growth, slow growth, and stable deformation. The growth rate of the strain is larger in the early loading stage, and the strain amount at this stage accounts for about 50% of the total strain. This is because the pores among gangue blocks are compacted in this stage, and the gangue block with large grain size is gradually broken. In the middle loading stage, the growth rate of the gangue strain decreases. At this stage, pores have been compacted, and the gangue deformation is mainly caused by fragmentation. In the later loading stage, the strain of the gangue remains stable. This is because the gangue cannot be broken, and has reached a relatively stable state.
- The maximum strain of the gangue is directly proportional to the loading rate, that is, the greater the loading rate, the greater the maximum strain. With the increase of loading rate, the maximum strain of the gangue increases from 0.321 to 0.353, indicating that the loading rate has a great impact on the mechanical properties and deformation characteristics of crushed gangue. The main reason is that under the low loading rate, the gangue fragmentation and compaction process are relatively slow, and a stable bonding of the gangue can be formed. At this time, the gangue cannot be further broken. Under the high loading rate, pores between the gangue are quickly compacted, and then the gangue with large particle size is quickly broken. At this time, the gangue is incapable of forming a stable bonding state. Finally, the gangue is crushed and compacted again, leading to a further increase of the strain.
- With the increase of loading rate, the maximum strain increases continuously. When the loading rate is greater than 2 kN/s, the growth rate of the strain decreases, indicating that 2 kN/s is the optimal loading rate under this condition. Therefore, when the backfill body is compacted, the optimal compacting force should be maintained at about 2 kN/s. Moreover, after the backfill body is backfilled into the goaf, the loading rate generated by the overlying surrounding rock is in a dynamic change under the disturbance of mining activities, which will have a greater impact on the bearing capacity of the backfill body. Consequently, the influence of mining activities should be minimized to reduce the disturbance to the backfill body.
- Porosity–strain relationship
- Porosity-stress relationship
3.2. AE Energy Characteristics of Gangue at Different Loading Rates
- The changing trend of the cumulative energy curves and strain curves are consistent. With the increase of loading rate, the cumulative AE energy of the gangue also increases. Through the AE monitoring technology, the dynamic monitoring of AE energy in the process of gangue fragmentation can reflect the damage process inside the specimen. It shows that AE energy can effectively characterize the mechanical properties of the gangue.
- When the loading rate is less than 1.0 kN/s, the AE energy and strain curve of the specimen can be clearly divided into three stages: early loading stage, middle loading stage, and later loading stage. In the early loading stage (Stage 1), strain and AE energy increase slowly. This is because the pores between the gangues are compacted, and the gangues are not broken under the low loading rate, and AE energy mainly stems from the friction between the gangues. In the middle loading stage (Stage 2), the crushing of gangue results in the release of a large amount of energy, which increases the accumulated energy rapidly. Due to the low loading rate, a stable structure can be easily formed by the gangue. Thus, the duration of the AE signal is short. In the later loading stage (Stage 3), the AE signal intensity is low, and the accumulated energy gradually tends to be stable.
- When the loading rate is more than 1.5 kN/s, the changing trend of AE signal energy at the early loading stage is the same as that under the low loading rate. However, at the middle loading stage, the gangue cannot adjust each other to form a stable carrier under the higher loading rate, some gangue is further crushed and accompanied by the energy release. This process lasts so long that the late stage of stress loading does not appear. The deformation process of gangue and the generation process of the AE phenomenon last for a long time, and the later loading stage (the accumulated AE energy tends to stable state) is not significant.
- As shown in Figure 6, the maximum AE energy of gangue specimens under six different loading rates during the whole compaction process are 1.1 × 103, 9.6 × 103, 10.8 × 103, 13.3 × 103, 14.3 × 103, and 14.4 × 103, respectively. Meanwhile, the cumulative energy of gangue specimens are 2.11 × 106, 14.32 × 106, 20.79 × 106, 24.18 × 106, 23.28 × 106, and 24.33 × 106, respectively. It is found that under the low loading rate, the damage of the gangue is smoother and the energy cycle is short, and the cumulative energy is also smaller; under the high loading rate, the gangue is broken, and the compaction process is more violent and the energy cycle is longer, the accumulated energy is greater.
3.3. Relationship Model of Macroscopic Deformation and AE Energy at Different Loading Rates
- The variation trend of maximum strain, maximum energy, and accumulated energy of gangue under different loading rates is consistent. With the increase of loading rate, the maximum strain, AE energy, and cumulative energy rapidly increase first and then become stable, but the fragmentation rate decreases. Other than that, when the loading rate is less than 1.5 kN/s, the change of the loading rate has a large impact on specimens; when the loading rate is more than 1.5 kN/s, the influence of the loading rate change on specimens is decreased.
- At the low loading rate, the relationship between the macroscopic deformation and energy change of gangue shows three stages, and the linear correlation coefficients at different stages are higher than 0.96. However, at the high loading rate, the relationship between macroscopic deformation of the specimens and AE energy is mainly reflected in the first two stages while the third stage is not obvious. It implies that the macroscopic deformation of gangue specimens is closely related to the change of energy, so the fragmentation process of gangue can be analyzed through the change of AE energy.
3.4. Distribution Characteristics of Force Chain of Gangue Model under Different Loading Rates
3.5. Fracture Evolution Characteristics of Gangue Model under Different Loading Rates
- Direct compression of pores under low stress is the main factor affecting macroscopic deformation of the gangue. The porosity of the gangue decreases with the decrease of residual height, and increases with the decrease of strain. The porosity is inversely proportional to the stress, and the decreasing rate decreases gradually.
- With the increase of loading rate, the maximum energy and cumulative energy of AE increase continuously, which is consistent with the macroscopic deformation characteristics of gangue. In the early loading, there is less gangue fragmentation and low AE signal; in the later loading stage, the gangue fragmentation is intensified, and the AE signal strength and cumulative energy increase significantly.
- With the increase of loading rate, the influence of loading rate on deformation, fragmentation and AE signals of gangue is gradually weakened.
- In the early loading stage, the distribution of the force chain and the fracture development of the gangue model are deepened. In the later loading stage, there is almost no difference in the state distribution of each model. The macroscopic deformation and failure mechanism of gangue under different loading rates is revealed from the mesoscopic point of view.
Data Availability Statement
Conflicts of Interest
- Li, J.; Huang, Y.; Gao, H.; Ouyang, S.; Guo, Y. Transparent characterization of spatial-temporal evolution of gangue solid wastes’ void structures during compression based on CT scanning. Powder Technol. 2020, 376, 477–485. [Google Scholar] [CrossRef]
- Guo, S.; Zhang, J.; Li, M.; Zhou, N.; Song, W.; Wang, Z.; Qi, S. A preliminary study of solid-waste coal gangue based biomineralization as eco-friendly underground backfill material: Material preparation and macro-micro analyses. Sci. Total Environ. 2021, 770, 145241. [Google Scholar] [CrossRef] [PubMed]
- Wang, J.; Zhang, J.; Zhang, Q.; Wu, Z.; Zhang, Q.; Wang, Y.; Gao, D. Analysis of the Control Effect and Parameter Optimisation of Urban Surface Deformation in Underground Coal Mining with Solid Backfilling. Adv. Civ. Eng. 2021, 2021, 6705685. [Google Scholar] [CrossRef]
- Yan, H.; Zhang, J.; Li, B.; Zhu, C. Crack propagation patterns and factors controlling complex crack network formation in coal bodies during tri-axial supercritical carbon dioxide fracturing. Fuel 2020, 286, 119381. [Google Scholar] [CrossRef]
- Huang, P.; Zhang, J.; Yan, X.; Spearing, A.J.S.; Li, M.; Liu, S. Deformation response of roof in solid backfilling coal mining based on viscoelastic properties of waste gangue. Int. J. Min. Sci. Technol. 2021, 31, 279–289. [Google Scholar] [CrossRef]
- Sun, Q.; Meng, G.; Sun, K.; Zhang, J. Physical simulation experiment on prevention and control of water inrush disaster by backfilling mining under aquifer. Environ. Earth Sci. 2020, 79, 429. [Google Scholar] [CrossRef]
- Shi, D.; Cao, D.; Xue, J.; Deng, Y.; Liang, Y. DEM studies on the effect of particle breakage on the critical state behaviours of granular soils under undrained shear conditions. Acta Geotech. 2022, 17, 4865–4885. [Google Scholar] [CrossRef]
- Cheng, Q.; Zhang, J.; Zhou, N.; Guo, Y.; Pan, S. Experimental Study on Unconfined Compression Strength of Polypropylene Fiber Reinforced Composite Cemented Clay. Crystals 2020, 10, 247. [Google Scholar] [CrossRef][Green Version]
- Kesimal, A.; Yilmaz, E.; Ercikdi, B.; Alp, I.; Deveci, H. Effect of properties of tailings and binder on the short-and long-term strength and stability of cemented paste backfill. Mater. Lett. 2005, 59, 3703–3709. [Google Scholar] [CrossRef]
- Zhou, N.; Han, X.; Zhang, J.; Li, M. Compressive deformation and energy dissipation of crushed coal gangue. Powder Technol. 2016, 297, 220–228. [Google Scholar] [CrossRef]
- Wu, D.; Luo, F.; Li, M.; Diao, Y.; Guo, Y.; Xu, P. Macroscopic and microscopic study on the compression bearing characteristics and deformation failure mechanism of gangue with different particle sizes. Powder Technol. 2021, 383, 198–211. [Google Scholar] [CrossRef]
- Xiao, M.; Ju, F.; Ning, P.; Li, K. Mechanical and Acoustic Emission Behavior of Gangue Concrete under Uniaxial Compression. Materials 2019, 12, 3318. [Google Scholar] [CrossRef][Green Version]
- Bi, H.; Ni, Z.; Tian, J.; Jiang, C.; Sun, H.; Lin, Q. Influence of lignin on coal gangue pyrolysis and gas emission based on multi-lump parallel reaction model and principal component analysis. Sci. Total Environ. 2022, 820, 153083. [Google Scholar] [CrossRef]
- Chen, T.; Fang, Q.; Wang, Z.; Zhu, W. Numerical simulation of compression breakage of spherical particle. Chem. Eng. Sci. 2017, 173, 443–454. [Google Scholar] [CrossRef]
- Meng, F.; Song, J.; Yue, Z.; Zhou, H.; Wang, X.; Wang, Z. Failure mechanisms and damage evolution of hard rock joints under high stress: Insights from PFC2D modeling. Eng. Anal. Bound. Elements 2021, 135, 394–411. [Google Scholar] [CrossRef]
- Gutiérrez-Ch, J.; Senent, S.; Melentijevic, S.; Jimenez, R. Distinct element method simulations of rock-concrete interfaces under different boundary conditions. Eng. Geol. 2018, 240, 123–139. [Google Scholar] [CrossRef]
- Liang, Z.; Trc, D.; Xl, B.; Lt, C. Acoustic emission, damage and cracking evolution of intact coal under compressive loads: Experimental and discrete element modelling. Eng. Fract. Mech. 2021, 252, 107690. [Google Scholar]
- Yan, Y.; Yang, C.; Peng, L.; Li, R.; Bai, H. Emission characteristics of volatile organic compounds from coal-, coal gangue-, and biomass-fired power plants in China. Atmospheric Environ. 2016, 143, 261–269. [Google Scholar] [CrossRef]
- Yang, B.Y.; Chen, Z.C.; Wu, F.H. The influence factors of sulfur emission of coal and coal gangue and the formation of acid rain. Environ. Chem. 2004, 23, 548–554. [Google Scholar]
- Feng, S.; Yan, Y.; Lai, C. Experimental study on flow boiling characteristics of hybrid micro-channels with gradient distribution pillars and bypass. Int. J. Heat Mass Transf. 2022, 186, 122468. [Google Scholar] [CrossRef]
- Ma, D.; Zhang, J.; Duan, H.; Huang, Y.; Li, M.; Sun, Q.; Zhou, N. Reutilization of gangue wastes in underground backfilling mining: Overburden aquifer protection. Chemosphere 2020, 264, 128400. [Google Scholar] [CrossRef] [PubMed]
- Zhou, H.; Zhang, M.; Sun, S.; Wang, X. Synthesis of Coal Gangue-Based Mesoporous X Zeolite with Soft Template and Its Adsorption Methylene Blue. Sci. Adv. Mater. 2021, 13, 2157–2166. [Google Scholar] [CrossRef]
- Liu, J.-P.; Li, Y.-H.; Xu, S.-D.; Xu, S.; Jin, C.-Y.; Liu, Z.-S. Moment tensor analysis of acoustic emission for cracking mechanisms in rock with a pre-cut circular hole under uniaxial compression. Eng. Fract. Mech. 2015, 135, 206–218. [Google Scholar] [CrossRef]
- Xu, X.; Xia, M.; Ke, F.; Bai, Y. Experimental Evidence of Critical Sensitivity in Catastrophe. Pure Appl. Geophys. 2006, 163, 1751–1767. [Google Scholar] [CrossRef][Green Version]
- Jiang, M.; Spikes, K.T. Estimation of reservoir properties of the Haynesville Shale by using rock-physics modelling and grid searching. Geophys. J. Int. 2013, 195, 315–329. [Google Scholar] [CrossRef][Green Version]
- Habr, B.; Saliba, Y.; Hajal, J.; Smayra, V.; Riachy, M.; Fares, N. Hydrocortisone mitigates ICU-AW by fine-tuning of muscle atrophic and hypertrophic signaling pathways in a sepsis model with limb immobilization. Life Sci. 2020, 261, 118366. [Google Scholar] [CrossRef]
- Munuera, C.; Barrena, E.; Ocal, C. Scanning force microscopy three-dimensional modes applied to conductivity measurements through linear-chain organic SAMS. Nanotechnology 2007, 18, 125505. [Google Scholar] [CrossRef]
|Loading Rate/(kN/s)||Stage 1||Stage 2||Stage 3|
|0.25||y = 9.288 x + 0.009||y = 13.209 x − 0.141||y = 2.639 x + 1.260|
|0.5||y = 4.747 x + 0.044||y = 94.252 x − 11.141||y = 25.233 x + 6.622|
|1.0||y = 11.592 x − 0.009||y = 50.115 x − 1.801||y = 6.128 x + 8.752|
|1.5||y = 11.881 x − 0.015||y = 75.086 x − 1.445|
|2.0||y = 22.670 x − 0.044||y = 72.071 x − 1.923|
|5.0||y = 12.298 x − 0.023||y = 75.696 x − 2.553|
Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations.
© 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).
Share and Cite
Qin, T.; Guo, X.; Huang, Y.; Wu, Z.; Qi, W.; Wang, H. Study on Macro-Meso Deformation Law and Acoustic Emission Characteristics of Granular Gangue under Different Loading Rates. Minerals 2022, 12, 1422. https://doi.org/10.3390/min12111422
Qin T, Guo X, Huang Y, Wu Z, Qi W, Wang H. Study on Macro-Meso Deformation Law and Acoustic Emission Characteristics of Granular Gangue under Different Loading Rates. Minerals. 2022; 12(11):1422. https://doi.org/10.3390/min12111422Chicago/Turabian Style
Qin, Tao, Xin Guo, Yanli Huang, Zhixiong Wu, Wenyue Qi, and Heng Wang. 2022. "Study on Macro-Meso Deformation Law and Acoustic Emission Characteristics of Granular Gangue under Different Loading Rates" Minerals 12, no. 11: 1422. https://doi.org/10.3390/min12111422